Presentation on theme: "2799.44599.86400.28200.610001.0 Mass (m/z) 6101.0 10 20 30 40 50 60 70 80 90 100 % Intensity MALDI-TOF-MS Sample Preparation for Synthetic Polymers via."— Presentation transcript:
2799.44599.86400.28200.610001.0 Mass (m/z) 6101.0 10 20 30 40 50 60 70 80 90 100 % Intensity MALDI-TOF-MS Sample Preparation for Synthetic Polymers via Nanoliter Induction Based Fluidic Deposition Brent Hilker 1 ; Kevin Clifford 1 ; Julie Harmon 1, Ted Gauthier 1,Andrew Sauter Jr. 2 ; Andrew Sauter III 2 1 University of South Florida, Tampa, FL; 2 Nanoliter, LLC, Henderson, NV Overview Purpose Evaluate Novel Nanoliter Induction Based Fluidics (IBF) versus Micropipette and Syringe Pump depositions for MALDI using dried droplet technique. Characterize selected polymers in each deposition method by: (M n ), (M w ), (PD), P SP, (S/N), Rs Deposition Homogeneity Methods Polystyrene (PS), poly(methyl methacrylate) (PMMA), poly(ethylene glycol) (PEG) were MALDI analyzed: With M n & M w ranging 2500-100,000 dA Homogeneity of deposition is classified using LEICA DMRX Cross polarization microscope Results Nanoliter IBF depositions Show increased S/N, Intensities, P SP More Accurate M n, M w, and PD values Greater homogeneity (sweet/hot-spot) of sample deposition Introduction The nanoliter wave, picture 1, makes use of induction based fluids (IBF) which is a novel technology that dispenses exact nanoliter volumes of solutions by electrokinetic means (1). IBF is green in its capacity to dispense small volumes, significantly reducing waste of highly toxic solvents and chemicals. Coupled with MALDI mass spectrometry using Ionic Liquid Matrices (ILM) IBF has been shown to improve results by making solutions homogeneous, resulting in greater signal-to-noise ratios (2). The induced charge on the droplet to be dispensed via IBF is correlated to surface area (3) and is soft showing no undesired electrochemistry on the analytes within the droplet (1-4). MALDI allows the rapid determination of: modal (M p ), molecular weight average (M n ), molecular number average (M n ), polydispersity (PD), and polymer spread (P sp ) (5). A comparison is made of IBF deposition method versus the micropipette and syringe pump which are all methods for solid matrix dried droplet (DD) depositions. DD depositions are known to be heterogeneous and this fact afflicts the reproducibility of the MALDI signal results It is well known that the more homogeneous samples exhibit improved reproducibility (6). Homogeneity was visually observed through the use of a LEICA DMRX cross polarization microscope Cross polarization images were obtained for sample DD depositions. Methods Poly(ethylene glycol) (PEG), poly(methyl methacrylate) (PMMA), and polystyrene (PS) are utilized in different recipes and molecular weights, figure 1, for (DD) deposition analysis. MALDI (DD) recipes were mixed in a [1:10:1] ratio, [Polymer: Matrix: Ion source] using tetrahydrofuran (THF) as solvent. Deposition volumes ranging from 500nl – 50nL are spotted for comparison using micropipette and nanoliter IBF device. Polymer Spectra for PEG and PS are obtained using a Voyager DE STR MALDI- TOF in linear mode. M n, M w, PD, P sp, signal to noise (S/N) at M p, resolution (Rs)are determined for PEG and PS for these MALDI spectra run on Voyager. A Brucker Autoflex MALDI-TOF in linear mode is used to determine S/N at M p for PMMA Results (cont.) Conclusion PS-TPB 2, table 1, exhibits S/N, Resolution (Rs), and intensity for decreasing volumes of IBF depositions. Table 2, shows that IBF 250nL is the optimum deposition size for PS-TPB 6 yielding the greatest S/N, Psp, and intensity. PEG 5 shows IBF 500nL depositions exhibit the greatest improvement in all categories of measurement, table 3. PMMA exhibits an increase in S/N and intensity at Mp, table 4. Table 5 shows an increase in S/N, intensity, Psp, and resolution for PS-TPB 99. References 1.Sauter, A. D. Precise Electrokinetic Delivery of Minute Volumes of Liquid(s). U.S. Patent 6,149,815, November 21, 2000. 2.Tu, T.; Sauter, A. D.; Gross, M. L. Improving the Signal Intensity and Sensitivity of MALDI Mass Spectrometry by Using Nanoliter Spots Deposited by Induction-based Fluidics.,2008. Doi:10.1016/j.jams.2008.03.017 3.Hilker,B.; Hilker, B.; Clifford, K.J.; Sauter, A.D,Jr.; Sauter, A.D.,III; Harmon J.P. The Delivery of Nanoliter Volumes via Induction Based Fluidics using Real Time Charge Measurements for Dispense Event and Volume Verification.(In Progress) 4.Sauter, A.D.,Jr. The Nanoliter Syringes. American Laboratory. February 2007. 5.Nielen, M. W.F.; MALDI Time-of-Flight Mass Spectrometry of Synthetic Polymers. J. Mass Spectrom. 1999, 18, 309-344. Acknowledgements We would like thank NIST for supplying some of the polymer standards used in this experiment. H. Lee Moffitt Cancer Center & Research Institute for supplying use of the Voyager DE STR MALDI. (PS-TPB 99) 5mg/mL Polystyrene(PS) (M n -92,600 M w 95,050 M p 94,400) 45mg/mL 1,1,4,4 Tetraphenyl-1,3 butadiene 5mg/mL AgTFA (PS-TPB 6) 5mg/mL Polystyrene (PS) (M n 5320) 45mg/mL 1,1,4,4 Tetraphenyl-1,3 butadiene 5mg/mL AgTFA (PMMA 10,600) 5mg/mL Polymethylmethacrylate (PMMA) (M n 10,600) 40mg/mL2,5-Dihydroxy benzoic acid (DHB) 5mg/mL NaTFA (PEG 5) 5mg/mL Poly (ethylene glycol) 40mg/mL Dithranol 5mg/mL NaTFA (PS-TPB 2) 5mg/mL Polystyrene (M n 2,300 M w 2514) 45mg/mL 1,1,4,4 Tetraphenyl-1,3 butadiene (TPB) 5mg/mL AgTFA Picture 1. Nanoliter IBF device Figure 1. Polymer recipes Figure 2b IBF 250nL MALDI Spectra (Raw Signal) PS-TPB-6 Figure 1a. Intensity comparison for PS-TPB-2Figure 1b IBF 100nL MALDI Spectra (Raw signal) PS-TPB-2 Table 1. PS-TPB 2 data 699.01759.22819.43879.64939.86000.0 Mass (m/z) 4.8E+4 10 20 30 40 50 60 70 80 90 100 % Intensity 2999.04099.45199.86300.27400.68501.0 Mass (m/z) 0 3186.6 0 10 20 30 40 50 60 70 80 90 100 % Intensity (PSTPB 2)MNMN MWMW PDP SP (S/N) M P Rs @ M P Laser ShotsIntensity M P IBF 500nL236125991.10116.9627233077501.80E+04 IBF 250nL225825451.12718.9631863207504.90E+04 IBF 100nL229925641.11518.943864.63317504.80E+04 MP 500nL241526401.09315.9520653217501.60E+04 MP 250nL233825941.10915.9818202577509.10E+03 (PS-TPB 6K) MNMN MWMW PDP SP (S/N) M P Rs @ M P Laser ShotsIntensity M P IBF 250nL658767331.022223147.54477506101 IBF 150nL651066541.022222.071113927504280 IBF 100nL650166441.021920.01126.65467503595 IBF 50nL640965721.025519.0348.34605001206 MP 500nL651766501.02051984.58527501142 MP 250nL646665981.02042087.28477501512 (PEG 5)MNMN MWMW PDP SP (S/N) M p Rs @ M p Laser shotsIntensity M P IBF 100nL537654191.0083230.13227501788 IBF 250nL537554181.0083128.33307501631.5 IBF 500nL537854181.007269514,5487503175 SP 100nL506951261.0113812.47407501529 MP 250nL517452161.0083518.66007501381 MP 500nL509951641.0134112.510487501192 PMMA 10.6 kDa(S/N) M p Intensity M p IBF 500nL121960 IBF 250nL11.83450 MP 500nL51260 MP 250nL5.81598 PS 99S/N M P Intensity M P Rs @ M P P SP IBF 100nL26.18967,83177 MP 100nL93955,21481 Results Table 2. (PS-TPB 6K) data Figure 2a. Intensity comparison for PS-TPB-2 Table 3. (PEG 5) data Figure 3a. Intensity comparison for PS-TPB-2 Figure 3b IBF 500nL MALDI Spectra (Raw Signal) (PEG 5) Image 1a PMMA cross polar IBF 100nL Image 1B PMMA cross polar MP 500nL Image 1c PS-TPB 99 cross polar IBF 100nL Image 1d PS-TPB-99 cross polar MP 100nL Table 4. (PMMA) data Table 5. PS 99 Data Figure 4. Intensity comparison for PPS-TPB- 99) A wide mass range of polymers and various MALDI recipe matrices are employed to evaluate the scope of use for the Nanoliter IBF device. These diverse variables subject this novel deposition method to real world scenarios that will be encountered in laboratories.
Your consent to our cookies if you continue to use this website.